2Introduction•CCorrosion i d i is degradation of materials’ properties d ti f t i l ’ ti due to interactions with their environments, and corrosion of most metals (and many materials for that matter) is inevitable.• Like death and taxes, corrosion is something we hope t avoid; b t ultimately it i something we h to id but lti t l is thi must learn to deal with.• The fundamental cause or driving force for all corrosion is the lowering of a system’s Gibbs energy.
3Types of Electrochemical Corrosion(1) Uniform or general corrosion.( ) U if l i(2) Galvanic or two-metal corrosion. two metal(3) Thermo galvanic corrosion.(4) Crevice corrosion, including deposit corrosion.(5) Pitting corrosion.(6) Inter granular and exfoliation corrosion corrosion. ………/Cont.
4Types of Electrochemical Corrosion(7) S l ti( ) Selective corrosion, selective l hi i l ti leaching.(8) Erosion corrosion.(9) Cavitation corrosion. Fretting corrosion.(10) Stress corrosion cracking.(11) C( ) Corrosion f i i fatigue.
51. Uniform or General Corrosion• In this form of corrosion, the attack is relatively evenly corrosion distributed all over the surface. It occurs typically under the following conditions: ▫ The material is a metal or alloy that is not liable to form protecting surface films in the environment in question, ▫ Electrochemical corrosion is the only deterioration process (which rules out cases of, e.g., erosion corrosion, where a mechanical process contributes), h i l ib ) ▫ The anodic and the cathodic reaction both occur all over the surface, but not at the same positions at the same moment (the two reactions may steadily change position) Closely position). connected to this is: That the concentration of the electrolyte does not vary significantly over the metal surface.
62. Galvanic Corrosion• Wh a more noble metal or alloy i i metallic When bl t l ll is in t lli contact with a less noble one, the corrosion rate of the latter is higher and that of the former is lower g than when the two materials are separated• A necessary condition for galvanic corrosion is that there is an electrolytic connection between the two metals• One of the most important factors in galvanic corrosion is the area ratio between the more noble i i th ti b t th bl and the less noble material. The larger this ratio is, the more intense is the galvanic corrosion.
73. Thermo-galvanic Corrosion• A temperature gradient i a material exposed to a di in i l d corrosive environment may cause a galvanic element and consequently lead to a form of corrosion called thermo-galvanic corrosion.• The hottest parts will normally act as dominating anodes with increased corrosion, while the colder parts are cathodic seats, which are protected.• It must be taken into account that the temperature may affect both the anodic and the cathodic reactions
84. Crevice or Deposit Corrosion• Thi is localized corrosion concentrated i crevices This i l li d i t t d in i or under dense deposits of corrosion products, dirt, sand, leaves and marine fouling. g• The crevice must be wide enough for liquid to penetrate into it. But, as a consequence of the mechanism, mechanism it must also be narrow; a condition for the corrosion to start is that the liquid in the crevice is depleted of oxygen.• Th liquid i th crevice must b stagnant and th The li id in the i t be t t d the diffusion of oxygen into the crevice must be slower than the consumption of O2 in the crevice ………/Cont.
94. Crevice or Deposit Corrosion• When crevice corrosion has been initiated the anodic reaction inside the crevice is mainly balanced by a cathodic reaction on the adjacent external surfaces. surfaces• The most typical cases of crevice corrosion are found on materials which are originally passive or easily passivated (e.g., stainless steels aluminum (e g steels, aluminum, unalloyed or low alloy steels in alkaline solutions), when these materials are exposed to dissolved, aggressive species like chlorides which can destroy chlorides, the passive oxide locally• Conventional stainless steels, such as AISI 316, 304, are liable to deposit corrosion in stagnant or slowly moving seawater. ………/Cont.
104. Crevice or Deposit Corrosion• A special type of crevice corrosion i the so- i l f i i is h called filiform corrosion, which may occur on steel, steel aluminum and magnesium underneath protecting films of more noble metals, lacquer, enamel or phosphates.
115. Pitting Corrosion• Pitting corrosion occurs on more or less passivated metals and alloys in corrosive media containing chloride, bromide, iodide or perchlorate ions.• Pitting potential depends on factors like material material, concentrations of aggressive species, pH and temperature.• The number and size of pits may vary greatly between different materials and from one area region to another on a given material.• Stainless steels (SS) have relatively high resistance y g against pit initiation and therefore, usually only few pits are formed. However, when a pit on SS has been formed it may grow rapidly, and the attack becomes serious
126. Inter granular (IC) & Exfoliation• Inter granular corrosion is localized attack on or at the grain boundaries (g.b), with little or no attack on other parts of the surface.• Thi is a dangerous form of corrosion, because th This i d f f i b the cohesion between grains can be reduced so much that tensile stresses cannot be transferred; the toughness of the material decreases markedly at a relatively early stage, and fracture can occur without warning.• A special form of corrosion in aluminum alloys is exfoliation corrosion, which usually propagates along the grain boundaries parallel to the surface. It is most familiar in AlCuMg alloys AlCuMg-alloys
137.Selective(SC)Corrosion(Leaching)• Selective corrosion occurs in alloys where one element is less noble than the others.• The less noble element is removed from the alloy, leaving a porous material of little strength and ductility ductility.• The most common example of SC is selective corrosion in brass, where Zn is dissolved and copper is left in place (dezincification).• The same corrosion forms and types may develop in aluminum bronzes (dealuminizing) in acids and strongly p polluted seawater.• Graphitizing of gray cast iron is another example of selective corrosion, in which iron is dissolved and graphite is left on the material.
148. Erosion Corrosion• When there i relative movement b h h is l i between the h corrosive medium and the metal, the metal surface is often affected by mechanical forces leading to increased corrosion denoted erosion corrosion.• Erosion corrosion is promoted by high velocities, liquid-gas and liquid-particle mixtures, and geometrical elements in the flow system, which lead to disturbance turbulence, and impingement. The turbulence impingement result is grooves and pits with a pattern determined by the flow direction and local flow conditions.
159. Cavitation Corrosion• Cavitation corrosion or rather called cavitation erosion corrosion, if the contribution of corrosion is small, is caused by high flow velocities and varying fluid dynamic conditions leading to rapid local pressure fluctuations.• It takes place in a wide range of equipment such as water turbines, pumps, propellers and on the external side of wet cylinder linings in diesel engines; the latter case is y g g ; due to vibration of the cylinder wall.• Cavitation damage is characterized by deep, narrow pits normal to the surface, localized close to each other or grown together over smaller or l h ll larger areas, often f leading to a spongy appearance. The edges of the pits are usually very sharp
16Fretting Corrosion• F tti corrosion t k place at th i t f Fretting i takes l t the interface b t between two parts, which are vibrating with very small amplitudes relative to each other.• Fretting corrosion i not to b considered as i i is be id d electrochemical corrosion. It can take place at ambient external temperature, just as the electrochemical forms.• Fretting corrosion is dependent on access of oxygen, but not of water.• Depending on the situation, fretting may cause seizing of p g , g y g originally movable components, and in other cases, loss of tolerances and loosening of parts that are considered fixed, e.g., pressed-on wheels. , g,p
1710.10 Stress CorrosionHydrogen Assisted Cracking• Stress corrosion cracking can be defined as crack formation and growth as a result of simultaneous static tensile stresses and corrosion.• Th tensile stresses may b due t external l di The t il t be d to t l loading, centrifugal forces or temperature differences, or they may be residual stresses caused by cold working, working welding or heat treatment. treatment• The cracks orientation is normal to the tensile stresses, may grow inter granularly or transgranularly, transgranularly and may be more or less branched branched.• If they are not detected in time, they will lead to rapid, unstable fracture.
1811. Corrosion Fatigue• Fatigue i a progressive cracking mechanism i is i ki h i which develops as a result of cyclic stress and which can potentially lead to major failures failures.• Fracture is failure under static loading from a stress raiser, at applied stresses below the yield raiser strength of the material.• Corrosion fatigue ( ) is crack formation and g (CF) growth due to simultaneous fluctuating stresses and corrosion. ………/Cont.
1911. Corrosion Fatigue• Just as f stress corrosion cracking, only the for i ki l h tensile stresses cause corrosion fatigue. The difference between these two deterioration forms is that one originates from static and the other from fluctuating stresses.• Any environment, which may cause some kind of surface corrosion, will cause CF when the stress conditions are present.
20Corrosion Under some SpecialEnvironment Conditions• A type of corrosion that occurs in soils and sometimes in water due to externally induced electric current is stray current corrosion.• A typical example is corrosion caused b current, t i l l i i d by t originating at an electric installation and flowing in and out of a buried pipeline.• diff different cause of corrosion on steel i soils i sulfate t f i t l in il is lf t reducing bacteria, which are operating under anaerobic conditions.• A th example of bi l i ll assisted corrosion i Another l f biologically i t d i is particularly experienced on more corrosion resistant materials, like stainless steels in seawater.
21References1. JM Drugli, E Bardal “Corrosion Detection and Diagnosis "Materials Science Engineering (2004)2. BA Shaw, RG Kelly “What is Corrosion?” Electrochemical Society Interface (2006)